Homologous Series of Rare-Earth Zinc Arsenides REZn2-xAs2.n(REAs) (RE= La-Nd, Sm;n= 3, 4, 5, 6)
Xinsong Lin; Arthur Mar; Inorganic Chemistry 52 (2013) 7261–7270; doi:10.1021/ic400933v

data_4335286
_publ_contact_author_address
; Department of Chemistry
  University of Alberta
  Edmonton, AB
  Canada  T6G 2G2
;
_publ_contact_author_email       arthur.mar@ualberta.ca
_publ_contact_author_fax         '(780) 492-8231'
_publ_contact_author_name        'Dr. Arthur Mar'
_publ_contact_author_phone       '(780) 492-5592'
_publ_section_title
;
 Homologous Series of Rare-Earth Zinc Arsenides REZn2-xAs2.n(REAs) (RE=
 La-Nd, Sm;n= 3, 4, 5, 6)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              7261
_journal_page_last               7270
_journal_paper_doi               10.1021/ic400933v
_journal_volume                  52
_journal_year                    2013
_chemical_formula_structural     'Ce6 Mn0.43 Zn1.28 As7'
_chemical_formula_sum            'As7 Ce6 Mn0.43 Zn1.28'
_chemical_formula_weight         1472.46
_chemical_name_common            'cerium zinc arsenide (6/0.4/1.3/7)'
_chemical_name_systematic        'cerium zinc arsenide (6/0.4/1.3/7)'
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   4.2821(8)
_cell_length_b                   4.2821(8)
_cell_length_c                   73.620(14)
_cell_measurement_reflns_used    786
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      29.86
_cell_measurement_theta_min      5.82
_cell_volume                     1169.1(4)
_computing_cell_refinement       'Bruker SAINT 7.68A (Bruker, 2009)'
_computing_data_collection       'Bruker SMART 5.054 (Bruker, 1999)'
_computing_data_reduction        'Bruker SAINT 7.68A'
_computing_molecular_graphics    'ATOMS 5.1 (Dowty, 1999)'
_computing_publication_material  'Bruker SHELXTL 6.12'
_computing_structure_refinement  'Bruker SHELXTL 6.12'
_computing_structure_solution    'Bruker SHELXTL 6.12'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Bruker PLATFORM/SMART APEX II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0646
_diffrn_reflns_av_sigmaI/netI    0.0321
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       110
_diffrn_reflns_limit_l_min       -111
_diffrn_reflns_number            5613
_diffrn_reflns_theta_full        33.24
_diffrn_reflns_theta_max         33.24
_diffrn_reflns_theta_min         1.66
_exptl_absorpt_coefficient_mu    34.114
_exptl_absorpt_correction_T_max  0.3591
_exptl_absorpt_correction_T_min  0.2142
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'Bruker SHELXTL 6.12 (Sheldrick, 2001)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.274
_exptl_crystal_description       irregular
_exptl_crystal_F_000             1884
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.02
_refine_diff_density_max         5.573
_refine_diff_density_min         -2.024
_refine_diff_density_rms         0.392
_refine_ls_extinction_coef       0.00015(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_matrix_type           full
_refine_ls_number_parameters     25
_refine_ls_number_reflns         685
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.059
_refine_ls_R_factor_all          0.0646
_refine_ls_R_factor_gt           0.0292
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0251P)^2^+7.9905P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0615
_refine_ls_wR_factor_ref         0.0721
_reflns_number_gt                437
_reflns_number_total             685
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            ic400933v_si_002_7.cif
_cod_data_source_block           ce6mn0.4zn1.3as7
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               4335286